Journal of Materials and Environmental Sciences ISSN : 2028-2508 CODEN : JMESCN
J. Mater. Environ. Sci., 2018, Volume 9, Issue 4, Page 1119-1128
Copyright © 2018, University of Mohammed Premier Oujda Morocco
Improvement of phenol removal from aqueous medium by adsorption on organically functionalized Moroccan stevensite M. Hamdaoui1, M. Hadri1,2, Z. Bencheqroun2, K. Draoui1,*, M. Nawdali3, H. Zaitan2,* A. Barhoun1 1
Laboratory MSI, Faculty of Sciences, Abdel Malek Essaadi University, B.P. 2121, M'hannech II, Tetouan, Morocco. Laboratory LCMC, Faculty of Science and Technology, Sidi Mohamed Ben Abdellah University, BP 2202, Fez, Morocco. 3 Laboratory LCMC, Polydisciplinary Faculty, Sidi Mohamed Ben Abdellah University, B.P 1223, Taza, Morocco.
Received 7 Aug 2017 Revised 17 Dec 2017 Accepted 21 Dec 2017 Keywords Phenol; Rhassoul; Surfactant; Hydrophobic interactions; Kinetic modeling; Adsorption isotherm. [email protected]
Abstract In this work, the adsorption of phenol on natural and organically modified Moroccan clay named Rhassoul was investigated using the batch equilibrium method. Several techniques, such as, X-ray fluorescence analysis (XRF), X-ray diffraction (XRD), Fourier transform infrared spectroscopy (FTIR) and thermal analysis (TGA/DTG) were used for clays characterization. Adsorption experiments were carried out varying initial phenol concentration, pH and contact equilibrium time. The adsorption isotherms of phenol on Rhassoul and modified Rhassoul by the HDTMA surfactant molecules were determined and modeled by Langmuir equation. The experimental results indicate that the adsorption was improved by increasing pH and initial concentration of phenol in the solution. Experimental and calculated kinetic data for equilibrium are well fitted with the pseudo second order kinetic model. The adsorption isotherm was described satisfactorily using the mathematical model of Langmuir with a maximum monolayer adsorption capacity of 25 mg.g-1 for organicallyRhassoul. The results indicate that raw and organically modified Rhassoul could be used as a low cost adsorbent in wastewater treatment for the elimination of phenolic compounds.
1. Introduction The industrial emissions cause serious degradation of the environment and damage to human health. Pollution of the environment is directly related to the economic development of civilization. It is a threat that is increasing and may affect both the natural balance and the human health. Phenolic compounds are among the most dangerous pollutants for human health and the environment. They have been classified as high-priority contaminants by the USA EPA (Environmental Protection Agency) . Phenol is mainly used as an intermediate in various industries (Refining petroleum, pharmaceuticals, plastics industry, production of dyes and pesticides...). The toxic and hazardous nature of phenols and their derivatives have been well documented [2-5] and can cause several health problems . The treatment of water contaminated with phenolic compounds remains a major challenge, especially for developing countries that have not yet all opportunities to integrate the concepts of sustainable development. The complexity of their chemical structure and the presence of aromatic rings, mean that the corresponding aqueous effluents require treatment in several steps. One of the most important steps is the adsorption process permitting the concentration of the compound in a solid phase. Some adsorbents commonly used on the removal of phenolic compounds by adsorption techniques are activated carbon, clays, zeolites, polymeric adsorbents, and some other low-cost materials [7-9]. These materials are very promising in this area. These adsorbents generally require subsequent specific treatment for the degradation of these molecules and regeneration of adsorbents [10-11]. The present investigation aims to study a simple and economic process for phenol removal from aqueous solution using low cost abundantly available adsorbent (natural or modified Rhassoul). The Rhassoul clay is characterized by a large cation exchange capacity CEC . This parameter is responsible for hydration of these mineral materials and subsequently for their hydrophilic properties. The intercalation of cationic surfactants in the clay galleries improves drastically the hydrophobic properties which play a key role in the retention of non-ionic organic pollutants. We used for this study the natural and modified Rhassoul by hexadecyltrimethylammonium bromide HDTMA: [N(CH3)3(C16H33)]Br. Batch experiments were carried out involving experimental parameters such as initial phenol concentration, pH and contact equilibrium time. Equilibrium and kinetic analysis were conducted to determine the factors controlling the rate of phenol adsorption. The optimization of the experimental parameters was achieved to find out the possibility of using this abundant material as low-cost adsorbent for phenolic compounds removal. Hamdaoui et al., J. Mater. Environ. Sci., 2018, 9 (4), pp. 1119-1127
2. Materials and methods 2.1. Materials The clay sample studied in this work was sampled from deposits in the careers of Tamdalet in East side of the Middle Atlas Mountains, Fez-Boulemane area, Morocco. The Moroccan natural clay, called locally Rhassoul, is a mineral product composed mostly of stevensite mineral [13-14]. This clay was modified by hexadecyltrimethylammonium bromide (HDTMA) as previously described [3, 15]. All chemicals used for analyses were reagent grade obtained from Sigma-Aldrich (Sigma-Aldrich Chimie S.a.r.l., Lyon, France). They were used without further purification. 2.2. Preparation of phenol solutions and organically modified Rhassoul by HDTMA Phenols solutions were prepared by dissolving the phenol in distilled water. The modified clay used in the experiments of the phenol adsorption, was prepared as follows: in a beaker using 200 ml of distilled water with 5g of natural Rhassoul and 0.375 g HDTMA for CEC reached saturation. After 2 h stirring at temperature of 60 °C, the suspensions were then centrifuged and intensively washed with distilled water until the total elimination of bromide ions as confirmed by AgNO3 test. The product obtained was filtered and dried at 50 °C in an oven for 24 hours. 2.3. Characterizations. 2.3.1 X-ray fluorescence (XRF). Elemental composition of the Rhassoul sample was determined by X-ray fluorescence (XRF) using a Bruker S4 Pioneer spectrometer. Total organic matter contained in the clay was analyzed by measurements of loss on ignition. 2.3.2 X-ray diffraction. Mineralogical composition of raw and modified clay was identified by powder X-ray diffraction analysis (XRD) using powder diffractometer model D8 Bruker, Bragg-Brentano geometry theta-theta, with a Lynxeye detector, autosampler nine positions for performing measurements to conventional angles (2θ> 4) but also at small angles (0.5°